A novel mechanical cleavage method for synthesizing few-layer graphenes
© Jayasena and Subbiah; licensee Springer. 2011
Received: 26 August 2010
Accepted: 19 January 2011
Published: 19 January 2011
A novel method to synthesize few layer graphene from bulk graphite by mechanical cleavage is presented here. The method involves the use of an ultrasharp single crystal diamond wedge to cleave a highly ordered pyrolytic graphite sample to generate the graphene layers. Cleaving is aided by the use of ultrasonic oscillations along the wedge. Characterization of the obtained layers shows that the process is able to synthesize graphene layers with an area of a few micrometers. Application of oscillation enhances the quality of the layers produced with the layers having a reduced crystallite size as determined from the Raman spectrum. Interesting edge structures are observed that needs further investigation.
There is an urgent need to develop a large-scale method to manufacture graphene reliably for various promising applications being developed . These applications rely largely on the unique properties of graphene [2, 3] and the properties are strongly affected by the method of synthesis . While several laboratory methods to synthesize graphene have been developed and reported, the suitability of these methods to large-scale manufacturing remains to be proven. These methods can be broadly classified as epitaxial growth, colloidal suspension, unconventional methods, and exfoliation. In the epitaxial growth method graphene can be grown on top of either metallic or insulator substrates using physical and chemical vapour deposition methods [2, 4, 5]. In the colloidal suspension method, a combination of aqueous or organic solvent with an initial raw material such as graphite oxide is used . There are also several unconventional methods such as unzipping carbon nanotubes (CNT), arc discharge, and detonation using chemicals that have been explored for graphene manufacturing. The unzipping of CNT can be categorized as an oxidizing method involving insertion of metal atoms with ammonia using thermal treatment, plasma cutting after embedding in polymer, and catalytic microwave cutting . The arc discharge method involves the use of a high-current arc discharge between a graphite anode and graphite cathode in a chamber filled with hydrogen and helium gas . In the detonation method, a mixture of natural graphite, nitric acid, and CH3NO2 is exploded in a vessel and graphene detected in the soot obtained . All these methods suffer from various limitations such as poor yield, use of special hazardous chemicals, and contamination of graphene with impurities or functional groups, and long processing time. The exfoliation method, the method of interest in this paper, essentially involves separation of graphene layers from bulk graphite; this technique can be further classified into thermal, chemical, or mechanical methods.
In thermal exfoliation, graphite (natural or graphite oxide) is used as the starting material and the process comprises of three steps: oxidization, thermal expansion/exfoliation and centrifugation, and ultrasonication . Chemical exfoliation is carried out at high temperatures and involves several process steps and chemicals . The devices can be fabricated on several surfaces, and deposition of graphene from solution is the main merit of this method. Mechanical exfoliation, the main focus of this paper, is another laboratory-based method for graphene sample preparation. The scotch tape method is the popular method of mechanical cleavage  that has been explored for separation of graphene. Repeated peeling is needed to achieve single layer graphene and it is difficult to predict the number of peelings required. Another micromechanical cleaving method reported by Ruoff et al  involves the use of an atomic force microscope (AFM) tip along with an array of highly ordered pyrolytic graphite (HOPG) mesas made from oxygen-plasma etching method. The HOPG islands were transferred to a SiO2/Si substrate using hydrofluoric acid. It is then manipulated using an AFM tip to obtain multiple layers of HOPG. A variation of this method involves gluing a block of prepared graphite to an AFM tip and scratched on Si substrates . In general, it is difficult to control the separation and number of graphene layers generated using these mechanical methods. In this context, there is further scope in exploring other mechanical exfoliation techniques for graphene synthesis with potential for low chemical usage and better process controllability. Application areas where ultrathin sectioning is routinely performed offer some ideas for mechanical exfoliation of layers from a bulk substrate.
Use of an ultrasharp wedge as a sectioning method has been used in biological sample preparation and ultrathin samples (as thin as 40 nm) are generated with either glass or diamond wedges . Mica, a layered material, was cleaved using a glass wedge proving the possibility of layer separation as early as in 1930 . Brittle and hard materials such as germanium have also been sectioned to nanometer-scale thickness using this technique . Reproducibility of section thickness, chemical inertness, and durability of the diamond wedge are the main advantages of this technique. Thus, there is potential in exploring the use of this technique in graphene synthesis as well.
Here, we adopt this sectioning technique to develop a novel mechanical exfoliation method to synthesize few layer graphene from bulk graphite. The method uses an ultrasharp single crystal diamond wedge to exfoliate a highly ordered pyrolytic graphite sample and generate the graphene layers. We test the effect of high-frequency oscillations applied along the wedge, which will enable a smooth sliding motion of the cleaved layers over the diamond wedge surface leading to better quality layers. The thickness of the layers obtained is analyzed using AFM and transmission electron microscopy (TEM) to study the layer structure and the edges in detail. The effect of applied oscillations is studied by calculating the crystallite size from Raman spectroscopic analysis.
Experimental setup and characterization methods
Results and Discussion
During every experimental run, it involved a series of 20 cleaving passes. During every pass, a layer is generated. As the wedge retracts and is ready for the next pass, the layer just generated remains adhered to the wedge surface. The subsequent cut generates another layer which pushes the previous layer further onto the wedge and subsequently on to the water bath. When the new layer goes underneath the previous layer or when the layer reaches the water surface, then in some cases curling of the layers was observed. More often than not a series of layers were observed floating on the water bath. The process is yet to be optimized and the current success rate in cleaving to obtain layers of 900 × 300-μm area is more than 50%.
Figure 4a shows an area where the sheet appears to be heavily crumpled. In the micrographs of layers obtained with application of oscillations, grain boundaries, folded graphene sheets, and smooth areas of the sheets are also clearly observed. No heavily crumpled regions were seen, but some structures that seem to resemble nanohorns can be observed (marked as 3 in the enlarged area), which needs further investigation. Nanohorns are considered as structures resulting from crushing of a single sheet of graphene . The large surface area of the nanohorns is reported to be useful in various applications such as hydrogen gas storage.
Raman spectroscopy data of the cleaved layers, produced with and without oscillation indicates several features such as the D band (information about defects), G band (in plane vibration) and 2D band (stacking order); these correlated well with reported data in the literature [3, 18]. There are no differences in the D band positions (1,332 cm-1) with and without oscillations. However, this D band position observed is different from that of bulk graphite (1,355 cm-1). The G band position was 1,577 cm-1 with oscillation and 1,578 cm-1 without. The Raman data is further analyzed using a curve fitting method involving deconvolution and fitting two Lorentzian functions, HOPG being a polycrystalline material .
The values of La calculated using this equation and experimentally obtained values of I D /I G are plotted as shown in Figure 7. It appears that La is smaller when ultrasonic oscillation is applied to the wedge. The value of La is inversely proportional to "amount of crystal boundary" and is a measure of dislocations, vacancies, as well as number of non-graphitic atoms, which in turn is proportional to chemical functionality and shear strength of linkages . The amount of disorder is an indication of fraction sp 2 bond and it is a measure of electrical, mechanical, and optical properties. The lower value of La when oscillations are applied indicates the improved the quality of the layers obtained. Also, higher the value of La, lower is said to be the shear strength and from Figure 7 we can conclude that shear strength tends to increase when ultrasonic oscillation used.
Conclusion and future work
We have demonstrated a novel mechanical cleavage technique to produce few layer graphene from bulk graphite using an ultrasharp diamond wedge assisted by ultrasonic oscillations. AFM measurements indicate that the proposed mechanical cleaving method is capable of producing thin layer graphene with a thickness of tens of nanometers. TEM studies reveal that there is considerable amount of attention required to understand the edge formation with ultrasonic oscillation usage since structures that seem to resemble nanohorns were observed. Application of ultrasonic vibrations along the tool edge is seen to significantly reduce the I D/I G ratios seen in a Raman spectrum. Hence, the applied oscillations may have potential to reduce the defects in cleaved layers. The application of ultrasonic vibration also reduces the crystallite size. In the future we will perform molecular dynamic simulations to understand the cleavage mechanism and the effect of process parameters on the cleavage.
Partial funding from NTU-MoE AcRF/Tier-1 RG11/07 grant is acknowledged. We thank Dr. G. A. J. Amaratunga (University of Cambridge) for the discussion on this topic and useful suggestions, during his visit to Nanyang Technological University (NTU). We also thank Dr. V. M. Murukeshan (NTU) for his valuable suggestions on formatting this paper.
- Stankovich S, Dikin DA, Dommett GHB, Kohlhaas KM, Zimney EJ, Stach EA, Piner RD, Nguyen ST, Ruoff RS: Graphene-based composite materials. Nature 2006, 442(7100):282–286. 10.1038/nature04969View ArticleGoogle Scholar
- Park S, Ruoff RS: Chemical methods for the production of graphenes. Nat Nanotechnol 2009, 4: 217–224. 10.1038/nnano.2009.58View ArticleGoogle Scholar
- Zhenhua Ni YW, Ting Yu, Zexiang Shen: Raman spectroscopy and imaging of graphene. Nano Res 2008, 1(4):273–291. 10.1007/s12274-008-8036-1View ArticleGoogle Scholar
- Allen MJ, Tung VC, Kaner RB: Honeycomb Carbon: A Review of Graphene. Chem Rev 2009, 110(1):132–145. 10.1021/cr900070dView ArticleGoogle Scholar
- Lee BJ, Yu HY, Jeong GH: Controlled Synthesis of Monolayer Graphene Toward Transparent Flexible Conductive Film Application. Nanoscale Res Lett 2010, 1–6.Google Scholar
- Janowska I, Ersen O, Jacob T, Vennégues P, Bégin D, Ledoux MJ, Pham-Huu C: Catalytic unzipping of carbon nanotubes to few-layer graphene sheets under microwaves irradiation. Appl Catal, A 2009, 371(1–2):22–30. 10.1016/j.apcata.2009.09.013View ArticleGoogle Scholar
- Subrahmanyam KS, Panchakarla LS, Govindaraj A, Rao CNR: Simple Method of Preparing Graphene Flakes by an Arc-Discharge Method. J Phys Chem C 2009, 113(11):4257–4259. 10.1021/jp900791yView ArticleGoogle Scholar
- Sun G, Li X, Qu Y, Wang X, Yan H, Zhang Y: Preparation and characterization of graphite nanosheets from detonation technique. MATER LETT 2008, 62(4–5):703–706. 10.1016/j.matlet.2007.06.035View ArticleGoogle Scholar
- Jin M, Jeong HK: Synthesis and systematic characterization of functionalized graphene sheets generated by thermal exfoliation at low temperature. J Phys D, Appl Phys (UK) 2010, 43(27):275402. 10.1088/0022-3727/43/27/275402View ArticleGoogle Scholar
- PU NW, Sung YU, Yih-Ming LIU, Ming-Der GER: Production of few-layer graphene by supercritical CO 2 exfoliation of graphite. 2009, 63(23):3.Google Scholar
- Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA: Electric Field Effect in Atomically Thin Carbon Films. Science 2004, 306(5696):666–669. 10.1126/science.1102896View ArticleGoogle Scholar
- Lu X, Yu M, Huang H, Ruoff RS: Tailoring graphite with the goal of achieving single sheets. Anglais 1999, 10: 269–272.Google Scholar
- Zhang YB, Small JP, Pontius WV, Kim P: Fabrication and electric-field-dependent transport measurements of mesoscopic graphite devices. Appl Phys Lett 2005., 86(7):
- Al-Amoudi A, Dubochet J, Gnaegi H, Lüthi W, Studer D: An oscillating cryo-knife reduces cutting-induced deformation of vitreous ultrathin sections. J Microsc (UK) 2003, 212(1):26–33. 10.1046/j.1365-2818.2003.01244.xView ArticleGoogle Scholar
- Obreimoff JW: The Splitting Strength of Mica. P ROY SOC LOND A MAT 1930, 127(805):290–297. 10.1098/rspa.1930.0058View ArticleGoogle Scholar
- Fernandezmoran H: A diamond knife for ultrathin sectioning. Exp Cell Res 1953, 5(1):255–256. 10.1016/0014-4827(53)90112-8View ArticleGoogle Scholar
- Wang H, Chhowalla M, Sano N, JIA S, Amaratunga JGA: Large-scale synthesis of single-walled carbon nanohorns by submerged arc. Anglais 2004, 15(5):5.Google Scholar
- Wang Yy, Ni Zh, Yu T, Shen ZX, Wang Hm, Wu Yh, Chen W, Shen Wee AT: Raman Studies of Monolayer Graphene: The Substrate Effect. J Phys Chem C 2008, 112(29):10637–10640. 10.1021/jp8008404View ArticleGoogle Scholar
- Jawhari T, Roid A, Casado J: Raman spectroscopic characterization of some commercially available carbon black materials. Carbon 1995, 33(11):1561–1565. 10.1016/0008-6223(95)00117-VView ArticleGoogle Scholar
- Tuinstra F, Koenig JL: Raman Spectrum of Graphite. J CHEM PHYS 1970, 53(3):1126–1130. 10.1063/1.1674108View ArticleGoogle Scholar
- Ferrari AC, Robertson J: Interpretation of Raman spectra of disordered and amorphous carbon. PHYS REV B 2000, 61(20):14095. 10.1103/PhysRevB.61.14095View ArticleGoogle Scholar
- Tuinstra F, Koenig JL: Characterization of Graphite Fiber Surfaces with Raman Spectroscopy. J COMPOS MATER 1970, 4(4):492–499.Google Scholar
- Cancado LG, Takai K, Enoki T, Endo M, Kim YA, Mizusaki H, Jorio A, Coelho LN, Magalhaes-Paniago R, Pimenta MA: General equation for the determination of the crystallite size La of nanographite by Raman spectroscopy. Appl Phys Lett 2006, 88(16):163106–163103. 10.1063/1.2196057View ArticleGoogle Scholar
- Nistor LC, Landuyt J, Ralchenko VG, Kononenko TV, Obraztsova ED, Strelnitsky VE: Direct observation of laser-induced crystallization of a-C:H films. APPL PHYS A-MATER 1994, 58(2):137–144. 10.1007/BF00332170View ArticleGoogle Scholar
- Beyssac O, Goff B, Chopin C, Rouzaud JN: Raman spectra of carbonaceous material in metasediments: a new geothermometer. Journal of Metamorphic Geology 2002, 20: 859–871. 10.1046/j.1525-1314.2002.00408.xView ArticleGoogle Scholar
- Nikiel L, Jagodzinski PW: Raman spectroscopic characterization of graphites: A re-evaluation of spectra/structure correlation. Carbon 1993, 31(8):1313–1317. 10.1016/0008-6223(93)90091-NView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.